1917] 
ZELLER—DURABILITY OF YELLOW PINE 
TABLE I (Continued) 
117 
I | ПІН |v уа мм гуп VU ike xxi XII 
Shortleaf pine (Pinus echinata) 
E1003 9 5.705 63 | 15.54 1.01 
E1004 я 6.252} .580115.9801 1.67 
Е1005 | 28.7 .078 | .594 | 16.839 | 1.40 
Е1006 ; 8.225| .628|17.732| 2.71 
Е1007 41 .109 | .609 | 16.579| 3.10 
F1001 | 29. 6.505 | .569 | 16.496 .05 | 2.56] 24. |23. | 2.75| .576 .04 
1002 | 29.1 |16.883| .580 | 16.883 | 0.00 
003 | 28.1 | 16.53 588 | 16.520 .06 
Е1004 5. 6.482| .578 | 16.475 ‚04 
1001 6 7.092 | .576 | 16.871} 1. 2.2 | 24. | 17. | 3.5 | S84 1.27 
G1002 | 29. 6.813 | .580 | 16.698 .68 
G1003 | 28. 6.480 | .588|16.265| 1.31 
G1004 | 28.2 |16.621| .589 | 16.338 | 1.70 
G1005 | 28.7 |16.770| .584 | 16.611 ‚95 
1006 | 28.4 | 16.659| .590 | 16.326 | 2.00 
(51007 | 29. 6.856| .581 | 16.693 ‚97 
H1001 .563 | .605 | 17.560 .0 2.14] 24. | 17. | 3.5 | .604 .36 
1002 5 .513 | .615 | 17.482 М 
Н 1003 6.965 | .606 | 16.792| 1.02 
1004 6.914 | .604 | 16.847 .40 
H1005 4 .251| .607 223 16 
006 203 | .607 185 ‚10 
007 6.540 | .586 | 16.431 .66 
I 1001 .510 | .611 | 18.500 ‚05 9 |25. | 15. | 3.79] 60) .68 
I 1002 ; .778 | .596 | 17.750 4 
І 1003 .085 | .606 | 16.980 А 
І 1004 | 28.: 4601 .617 2314 1.2 
І 1007 | 30. .220| .607|17.978| 1.3 
А1101 | 27.5 4281 .670|17.263| 6.31 | 22.98] 16. | 14. | .5 | .674| 5.90 
А1102 d .597| .671 .392| 6.49 
A1103 | 28. .594 | .663|17.427| 6.27 
А1104 | 28.7 .881| .657| 17.742 | 6.03 
А1105 | 28. .837| .708 | 18.964 | 4. 
А1106 .2 | 26.795 | .950 | 24.380 | 9.02 
В1101 | 28.2 | 19.295 | .684 | 18.378 | 4.75 | 20.32] 16. | 12. | .5 | .666 3.92 
В1102 - 8.223| .652 .580| 3.53 
B1103 9 8.525| .664 .818| 3.82 
B1104 Е 9.242 | .664 | 18.560| 3.54 
C1101 | 30. 7.865 | .595 .260 | 3.39 | 18.5 | 16. | 13. | .5 | 646 3.84 
С1102 | 30.1 .890| .594 | 17.740 | .84 
C1103 ‚9 .519 | .653 .551| 4.96 
C1104 5 .693 | .744 .290| 6. 
01101 | 29.5 .353 | .690 | 18.599 | 8.62 | 21.04 16. | 17. | .5 | .682 8.68 
01102 7 .956 | .696 .279 | 8.40 
D1103 5 .127 | 672 .789 | 7.00 
01104 D .940| .683 haat ФА 
D1105 3 1101 .676 383) 9. 
D1106 Ы .445 | .677 | 17.498 | 10. 
1 E1102 yo 6.715 | .587 | 15.494| 7.30 |{14.32| 10. | 32. | 1.5 | .526| 5.36 
1 E1103 ‚2 5.424 | .528 | 14.250| 7.60 |* 3.68 
1 E1104 : 4.660} .488 | 14.398 | 1.79 
ТЕ = 5.078 | .502 | 14.360} 4.76 
“wood. 
; Partaly sap-woo 
{ Percentage of resin in heart-wood where both heart-wood and sap-wood occur 
in the same е block. 
